**HAL Id: hal-00685222**

**https://hal.archives-ouvertes.fr/hal-00685222**

Submitted on 4 Apr 2012
**HAL is a multi-disciplinary open access**
archive for the deposit and dissemination of
sci-entific research documents, whether they are
pub-lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.

**L’archive ouverte pluridisciplinaire HAL, est**
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.

**Simulation of NMR Fermi contact shifts for Lithium**

**battery materials: the need of an eﬀicient hybrid**

**functional approach**

### Yuesheng Zhang, Aurore Castets, Dany Carlier, Michel Ménétrier, Florent

### Boucher

**To cite this version:**

Yuesheng Zhang, Aurore Castets, Dany Carlier, Michel Ménétrier, Florent Boucher. Simulation of NMR Fermi contact shifts for Lithium battery materials: the need of an eﬀicient hybrid functional approach. Journal of Physical Chemistry C, American Chemical Society, 2012, 116 (33), pp.17393-17402. �10.1021/jp304762f�. �hal-00685222�

**Simulation of NMR Fermi contact shifts for Lithium battery **

**materials: the need of an efficient hybrid functional approach **

Yuesheng Zhang,1 Aurore Castets,2,3 Dany Carlier,2,3 Michel Ménétrier,2,3 and Florent
Boucher1*

1_{Institut des Matériaux Jean Rouxel (IMN), Université de Nantes, CNRS, }
2 rue de la Houssinière, BP 32229, 44322 Nantes Cedex (France)

2_{CNRS, Université de Bordeaux, ICMCB, }

87 avenue du Dr. A. Schweitzer, 33608 Pessac Cedex (France)
3_{CNRS, IPB-ENSCBP, ICMCB, }

87 avenue du Dr. A. Schweitzer, 33608 Pessac Cedex (France) Received April, xxx 2012

In the context of the development of NMR Fermi contact shift calculations for assisting
structural characterization of battery materials, we propose an accurate, efficient, and
robust approach based on the use of an all electron method. The full-potential linearized
augmented plane wave method, as implemented in the WIEN2k code, is coupled with
the use of hybrid functionals for the evaluation of hyperfine field quantities. The
WIEN2k code is able to fully relax relativistic core states and uses an autoadaptive
basis set that is highly accurate for the determination of the hyperfine field.
Furthermore, the way hybrid functional approaches are implemented offers the
possibility to use them at no additional computational cost. In this paper, NMR Fermi
contact shifts for lithium are studied in different classes of paramagnetic materials that
*present an interest in the field of Li-ion batteries: olivine LiMPO*4* (M = Mn, Fe, Co, Ni), *
anti-NASICON type Li3*M*2(PO4)3* (M = Fe, V), and antifluorite-type Li*6CoO4. Making
use of the possibility to apply partial hybrid functionals either only on the magnetic
atom or also on the anionic species, we evidence the role played by oxygen atoms on
polarisation mechanisms. Our method is quite general for an application on various
types of materials.

PACS : 76.60.-k, 71.15.Mb

I. INTRODUCTION

In the context of finding new and efficient electrochemical energy storage solutions,

important efforts have been devoted to the study of transition metal (TM) compounds

as materials for positive electrodes in Li ion batteries.1 In this highly competitive and

strongly applied research domain, there is still an important need in having a very good

knowledge of the bonding properties of the active material together with information

on its crystal structure and/or local structure organization. On the latter point, solid state

magic angle spinning nuclear magnetic resonance (MAS-NMR) is a very powerful and

accurate technique that is now widely used for studying electrode materials. Relevant

examples can be found in Ref. 2-8 where 7Li or 6Li MAS-NMR is used to study Li

environment in battery materials.

Due to the hyperfine interactions between the nuclear magnetic moment of Li and the

electronic spin density induced by paramagnetic TM ions, the NMR shift of Li nucleus

in Li-TM compounds is often largely different from that in diamagnetic environments.

Hyperfine interactions consist of through space dipolar interactions and a through bond

Fermi contact one. For Li-TM oxide compounds considered here, the Li MAS-NMR

shift is mainly determined by the isotropic Fermi contact interaction which is due to the

presence of electron spin density on the Li nucleus, as transferred from the orbitals of

neighboring paramagnetic species. When different NMR signals are observed in

concordance with the existence of more than one Li environment, it becomes crucial to

correctly assign those NMR peaks. When paramagnetic compounds are submitted to an

the population of the two spin channels: the majority one (up, aligned with the applied

field) and the minority one (down). Two basic mechanisms have been proposed to

account for the transfer of electron spin density inducing the Fermi contact shift in

lithium transition metal compounds: spin delocalization and spin polarization.9 The

delocalization mechanism corresponds to transfer of unpaired electron spin density

*from a TM d orbital to the Li nucleus with the same polarity (up) by orbital overlaps, *

either directly or via oxygen. This leads to a positive NMR shift on the Li nucleus. The

spin polarization mechanism corresponds to the polarization of a fully occupied (either

*d cationic or p anionic) orbital induced by unpaired electrons in the d orbital of the TM *

ion. Due to the presence of spin polarized partially occupied d orbitals, mixing

*interactions between the anionic p and cationic d levels are different on the majority *

(up) and minority (down) spin channels. This induces a negative spin polarization for

the occupied orbitals which can be transferred to Li again either directly or via oxygen

depending on the geometry. Consequently, a negative NMR shift on Li ion is observed

when such polarization occurs. This mechanism will be discussed in detail in a

forthcoming paper. The occurrence and the relative importance of these delocalization

and polarization mechanisms depend on the spin state of transition metal ions and the

local environment of the Li ion. An analysis based on these two mechanisms can be

used to qualitatively assign the lithium NMR signals in simple cases, but it remains

difficult for compounds with complicated structure or when only small differences

between different signals exist. Hence, theoretical calculations are very helpful for this

qualitative approach based on plane wave/pseudo-potential calculation was thus

introduced to investigate the transfer mechanisms. Furthermore, the assignment of the

NMR peaks in a given compound was correlated to the integrated spin density found in

a sphere around Li. However, as shown below this method suffers from some

limitations and, in some cases, correct assignment of NMR shifts requires the

calculation of the Fermi contact shift.

If the paramagnetic behavior of the compound obeys ideal Curie law (spin only), the

Fermi contact shift of the probed nucleus (lithium for instance) can be expressed as:11

2
0
( 1)
3 3
*eff theory*
*i* *i* *i*
*i* *e* *B* *M Curie*
*con* *i* *i* *i*
*e* *B* *A* *e* *B*
*g* *S S*
*A* *A* *A*
*kT* *g* *kT* *N* *g*
μ
μ χ
δ
γ γ μ γ μ μ
− −
+
= = =
= = = (1)

*where S is the total spin quantum number of the paramagnetic ions, ge* is the free

*electron g factor, μB is the Bohr magneton, μ0 is the magnetic permeability in vacuum, γi*

*is the gyromagnetic ratio of the probed nucleus, ħ is the reduced Plank constant, k is *
*Boltzman constant, χM-Curie* is the Curie-like theoretical molar magnetic susceptibility,

*theory*
*eff*−

μ *is the theoretical magnetic moment, NA is Avogadro’s number, and T is the *

*temperature. Ai* is the isotropic hyperfine coupling constant, which is related to the
portion of the global magnetization that is present at the nucleus site:

0 _{(0)}
3
*i* *i* *i*
*e* *B* *HFF*
*A* *g*
*S*

### μ

### γ

### μ ρ

= = (2) where*i*(0)

*HFF*

ρ is the electron spin density averaged inside the Thomson sphere and has been used by many authors for the calculation of hyperfine field:12-14

8
(0)
3
*i* *i*
*B* *HFF*
*HFF* =

### π μ ρ

(3)Whereas Eq. (1) has been used recently by Mali et al. for the calculation of the Fermi

contact shift in orthosilicate positive electrode materials,15,16 the experimental magnetic

susceptibility often deviates from the theoretical Curie-type susceptibility due to

possible orbital contribution and/or residual magnetic correlations. In such situation,

the Fermi contact shift can be calculated using either the experimental effective

magnetic moment or the magnetic susceptibility as:

(*i*) if a Curie-Weiss behavior is obeyed

exp
2
3 ( )
*eff*
*i*
*i*
*con* *i*
*e* *B*
*A*
*g* *k T*
μ
δ
γ μ
−
=
− Θ
= (4a)
(*ii*) in a general case
exp
0
*i*
*M*
*i*
*con* *i*
*A* *e* *B*
*A*
*N* *g*
χ
δ
γ μ μ
−
=
= (4b)

*where χM-exp* is the experimental molar magnetic susceptibility, μ_{eff}_{−}_{exp} is the
*experimental effective magnetic moment, Θ is the Weiss constant. *

A recent paper of Kim et al.17 clearly recommends the use of the experimentally

determined Curie-Weiss parameters to calculate the Fermi contact shift, which is also

supported by our previous calculations.18 Moreover, we showed that for cases where

the magnetic behavior is not Curie-Weiss type at the temperature of the NMR

measurements, one should preferably use the experimental susceptibility at this

temperature to calculate the NMR shift.19 Therefore, in the present paper, we will only

deal with Fermi contact shift values calculated with Eqs. (4a) or (4b) depending of the

applicability of the Curie-Weiss law or the knowledge of the experimental

sample during the NMR measurement with which we wish to make a comparison.

Based on the details of the NMR measurements, this temperature was estimated as

stated in each case.

Assuming that the magnetic susceptibility is known, the other key quantity that enters

*Eq. (4b) for the calculation of Fermi contact is the hyperfine coupling constants Ai* for

which an accurate knowledge of *i* (0)

*HFF*

ρ is needed. Many calculations of Fermi contact coupling constants of atoms or molecules have been performed with post

Hartree-Fock theory using molecular approaches.20-24 Those results showed that it is a

great challenge to obtain a good agreement between calculations and experiments, the

accuracy of these calculations being very much dependent of the basis set completeness

and of the correlation level. Pretty good agreement between experimental and

theoretical values can be obtained using high level post Hartree-Fock methods coupled

with extended basis sets.22-24 Unfortunately, such calculations are limited to small

molecular or cluster systems due to the large cost of such computations. In recent years,

Density Functional Theory (DFT) has been considered as a good alternative to post

Hartree-Fock methods for the calculation of Fermi contact coupling constants as it

requires a much lower computational cost. Many examples of applications can be found

on molecular systems with lots of tests and developments using various

exchange/correlation functionals or for improving the basis set.25-31 Concerning the

study of crystalline compounds, people in the context of Mössbauer or ESR

spectroscopies were traditionally more interested in the hyperfine field (HFF) which is

While all-electrons methods are still the reference ones when periodic boundary

conditions need to be applied,12,32-35 pseudo-potential approaches have recently

demonstrated their efficiency for the calculation of *i* (0)

*HFF*

ρ .36 This is related to the development of the PAW implementation37 and, in addition, the possibility to take into

account the core states relaxation.38-40

In DFT calculations, the quantum correlation effect (exchange and correlation

interaction) between electrons is taken into account explicitly (though approximately),

which is important for the calculation of hyperfine coupling constants. However, the

exact form of exchange-correlation potential in DFT is unknown, so approximations

have to be made for DFT to become a practical tool. The local density approximation

(LDA) and generalized gradient approximation (GGA) to the exchange-correlation

potential have been widely used in DFT calculations. However, there is one basic

deficiency in LDA or GGA: the self interaction error (SIE) of each electron in the

Hartree term is not completely canceled by the exchange-correlation term. There is no

such error in Hartree-Fock theory because this self interaction can be exactly canceled

by the Fock exchange interaction term (“exact” exchange potential). The SIE has a

*large effect on localized transition-metal d or rare earth f orbitals, hence LDA or GGA *

is not appropriate to describe these orbitals. To overcome this deficiency, many

*methods have been proposed. One is the “GGA+U”. In this approach, Hubbard type *

*interaction is added to localized d or f electrons.*41 The other method that is now widely

replaced by Fock-type exact exchange potential to remove the self interaction error.42

*Thus, a better description for localized d or f orbitals can be expected from it. *

*In order to obtain correct hyperfine coupling constants Ai*, we need a method that can

accurately describe the valence states but also the semi-core and core states very close

to the nucleus. Mali et al. have calculated hyperfine coupling constants of Li2MnSiO4

polymorphs with the Quantum Espresso package. They used standard GGA for the

exchange correlation potential, a plane wave basis set coupled with norm-conserving

pseudopotentials, and the PAW development implemented in the “GIPAW package”

for recovering all-electrons properties but apparently no core states relaxation. NMR

Fermi contact shifts were calculated by assuming an ideal Curie behavior (Eq. (1)) at

room temperature.15,16 Kim et al. have adopted a more accurate and robust approach for

studying several paramagnetic Fe(III) phosphates.17 They have used an all-electron

linear combination of atomic orbitals (LCAO) in the Crystal06 code together with

hybrid functional method to calculate the spin density at the nucleus. NMR Fermi

contact shifts were then obtained considering experimental Curie-Weiss type behaviors

(Eq. (4a)). Such an approach is however very computer-demanding as the Fermi

contact shift calculation requires large basis sets for having a good accuracy.

In the present paper, we selected the full-potential linearized augmented plane wave

(FP-LAPW) method implemented into the WIEN2k code to perform the calculations,43

as we recently did for several tavorite-like LiMPO4.OH and MPO4.H2O phases.18,19

The full-potential linearized augmented plane wave (FP-LAPW) method is usually

compounds. Contrary to an LCAO method, the Full Potential WIEN2k/LAPW method

uses an adaptive basis set whose completeness can be easily evaluated. Furthermore,

the possibility to use a fully relativistic basis set has demonstrated its interest in the

determination of nuclear properties like HFF13 (or ρ*HFF*(0), Eq. (3)) which is obtained
by averaging spin density inside the nuclear Thomson sphere.12 Beside the standard

*GGA method, we also evaluated the performance of GGA+U and hybrid functional *

methods within this code. In WIEN2k, the unit cell is divided into (1) non-overlapping

*atomic spheres centered at the atomic sites and (2) an interstitial region. The “U” term *

*in GGA+U is applied to localized d or f orbitals, only inside the corresponding atomic *

*spheres. This is the general way to perform the GGA+U calculation. For hybrid *

functional calculations, the situation is more complex. The partial exchange potential is

usually applied in the whole unit cell, but in WIEN2k, the implementation of hybrid

*functional methods uses a similar strategy as that of GGA+U. Therefore, partial exact *

exchange potential is also applied inside the selected atomic spheres only, which makes

*its calculation cost comparable with that of GGA or GGA+U, and its result to be similar *

*with GGA+U to some extent. *

In this article, we have selected several Li transition-metal compounds to calculate

*the Fermi contact shift of the Li nucleus. First, we selected the LiMPO*4* (M=Mn, Fe, Co, *

*Ni) phosphates with olivine structure. There is only one kind of Li site in LiMPO*4, and

the experimental Fermi contact shifts for Li are positive (Mn) and negative (Fe, Co and

Ni), respectively.3 Second is the antifluorite-type Li6CoO4. The Fermi contact shifts of

Here we will present quantitative results and compare them with the previous ones.

Finally, the monoclinic Li3Fe2(PO4)3 and Li3V2(PO4)3 phases are discussed. The Fermi

contact shifts of the three Li ions in Li3V2(PO4)3 have been measured by Cahill et al.,6

and that of Li3Fe2(PO4)3 have been measured by Davis et al.,7 and simultaneously by

some of us.10 The Fermi contact shifts and mechanisms in these two compounds have

been qualitatively modeled by some of us.10 This will allow us to point out the

limitations of the earlier qualitative method.

II. COMPUTATIONAL DETAILS

Before calculating ρ*HFF*(0) (or HFF) with the WIEN2k code, the crystal structure of
every compound has been fully relaxed with the Vienna ab initio Simulation Package

(VASP),44-46 using the experimental crystal structure as a starting point. Relaxations

have been carried out using the PBE-type GGA47 for the exchange correlation potential

and all the ρ* _{HFF}*(0) calculations obtained afterwards with different functionals (GGA,
GGA+U, Hybrid) are performed on these optimized structures. By this way, we can

directly compare the effect of different exchange-correlation potentials on the spin

transfer mechanism keeping the structural features unchanged. Bonding and electronic

structure analysis can be done afterwards and will be detailed on a forthcoming paper.48

To test the validity of our calculations, HFF were also calculated on structures relaxed

within the GGA+U formalism. In most cases, the conclusions obtained with these two

different sets of structures are similar, hence only the results obtained by the former

methodology (GGA relaxation) are included in this paper. The relaxation has been

package, a plane wave energy cut-off of 600eV and a k-mesh dense enough to reach the

convergence.

For the ρ*HFF*(0) calculations with WIEN2k, the spherical radii of atoms have been
chosen in such a way that those spheres are nearly touching in the unit cell. The number

of k-points in the Brillouin zone and the energy cutoff have been chosen to ensure the

convergence of total energy, charge and spin density ρ*HFF*(0). Thus, the parameters
*used in the calculation are (1) LiMPO*4* (M=Mn, Fe, Co, Ni): RminKmax *≈ 7.0; atomic
*spheres radii of Li, P and M(Mn, Fe, Co, Ni) are 1.87, 1.61 and 2.0 a.u., respectively; *

*atomic sphere radii of O in M=Mn, Fe, Co, Ni are 1.3, 1.26, 1.3, 1.27 a.u., respectively; *

47 irreducible k-points with a (5×9×11) k-point mesh ; (2) Li6CoO4*: RminKmax*=7.6, 90

irreducible k-points with a (9×9×12) k-point mesh, atomic spheres of Li, Co and O are

1.87, 1.99 and 1.7 a.u., respectively; (3) Li3*M*2(PO4)3 *(M=Fe, V): RminKmax *= 6.9; 24

irreducible k-points with a (5×3×5) k-point mesh; the atomic spheres of Li, V, P and O

in V case are 1.80, 1.87, 1.44 and 1.44 a.u., respectively; while the atomic spheres of Li,

Fe, P and O in Fe case are 1.81, 1.89, 1.42 and 1.42 a.u., respectively.

As mentioned previously, the purpose of this study is to quantitatively evaluate NMR

Fermi contact shifts in order to discuss on the performance of various functional for the

accurate description of the ρ* _{HFF}*(0). Therefore, we chose a set of compounds
presenting different spin transfer mechanisms. Beside standard PBE/GGA approach,

*GGA+U and hybrid functional methods were tested. The Hubbard U correction was *

*applied on the TM-3d orbitals using the formalism introduced by Anisimov et al.*49 The

*variable in the calculation. Only an effective value U*eff*=U-J is used in the present *

*GGA+U method, where U is the on site electron-electron repulsion and J is the *

exchange interaction. Concerning hybrid functionals, there are many kinds of them in

the literature, such as PBE0, B3LYP, B3PW91, HSE, etc., and every method contains a

fixed weight of exact exchange potential. However, the suitable ratio of exact exchange

potential to be applied depends on the system. Thus, it is not easy to get good results for

all compounds with a fixed weight of exact exchange potential, especially for the

calculation of Fermi contact shifts, which are subtly dependent on the electronic states

of neighboring ions. Here, we therefore adopt the PBE-Fock-α method for the hybrid

functional calculations. In this method, the weight of exact exchange potential can be

*controlled by the fractional variable α. *

The exchange-correlation potential *PBE−Fock*−α

*xc*

*E* is calculated as:

### [ ]

## (

### [

### ]

### [

### ]

## )

*PBE Fock* *PBE* *HF* *PBE*

*xc* *xc* *x* *corr* *x* *corr*

*E* − −α _{=}*E*

_{ρ α}

_{+}

*E*

_{ψ}

_{−}

*E*

_{ρ}

_{(5) }

where *PBE*

### [ ]

ρ*xc*

*E* is the PBE exchange-correlation potential of the system, *ExHF*

### [ ]

ψ*corr*

and *PBE*

### [

### ]

*x*

*corr*

*E* ρ are exact and PBE-type exchange potential of the corresponding
orbitals.

In the WIEN2k code, the exact-exchange/hybrid methods are implemented only

inside the atomic spheres and traditionally for the localized electrons. However, as we

have mentioned above, the oxygen ion may play an important role in the spin transfer

from the TM ions to the Li nucleus, via both spin delocalization and spin polarization

mechanisms. To take this into account, we have also applied the Fock correction to

Functional calculations in this paper: in the first case, the partial GGA exchange

*potential of the sole transition-metal 3d orbitals inside the corresponding atomic *

spheres is replaced by the corresponding exact potential (Hybrid Functional I: HyF1)

*and in the other case the partial GGA exchange potential of transition-metal 3d and *

*O-2p orbitals in the corresponding atomic spheres are both replaced by the *

corresponding exact potential (Hybrid Functional II: HyF2). This distinction is

important in the calculation as we will see in the following. Furthermore, partial GGA

exchange potential of other atoms in the unit cell can also be replaced by exact

*exchange potential besides transition-metal 3d and O-2p orbitals, but the results show *

that there is no improvement in this calculation when compared to HyF2 kind of

calculation (as illustrated for selected examples in the supplementary information,

Table S-I).

III. RESULTS AND DISCUSSSION

*A. Study of LiMPO*4 *phases (M=Mn, Fe, Co, Ni) *

*Olivine LiMPO*4* phases crystallize in the Pnma space group, and consist of distorted *

LiO6*, MO*6 and PO4 units. The phosphorous ions occupy tetrahedral sites, while the

lithium and transition-metal ions occupy octahedral sites. There is only one kind of

*lithium ion site (4a site) in LiMPO*4 compounds. Every LiO6 octahedron shares edges

*with two MO*6* octahedra and corners with four other MO*6 polyhedra (Fig. 1). The

experimental crystal parameters are: (LiMnPO4: a=10.431 Å, b=6.0947 Å,

c=4.7366 Å),50 (LiFePO4: a=10.338 Å, b=6.011 Å, c=4.695 Å),51 (LiCoPO4:

c=4.6763 Å).50_{ The transition metal ions in these compounds are divalent: High }

Spin(HS)-Mn2+ *(3d*5*: t2g3eg2, S=5/2), HS-Fe*2+ *(3d*6*: t2g4eg2, S=2), HS-Co*2+ *(3d*7*: t2g5eg2 , *

*S=3/2) and Ni*2+ *(3d*8*: t2g6eg2, S=1). For convenience, here we still use the term “t2g*”and

*“eg” to denote electrons in different d orbitals of M ions though it is not strictly correct *

*because of the distortion of MO*6 octahedra. Note that we also adopt the usual

denomination “eg” for the strictly speaking eg* antibonding hybrid orbital with oxygen.

The experimental room temperature NMR Fermi contact shifts of 7Li at 310 K,

effective magnetic moments and Weiss constant for LiMnPO4,LiFePO4, LiCoPO4 and

LiNiPO4 *are (68 ppm, 5.4 μB, -58 K), (-8 ppm, 6.8 μB, -161 K), (-86 ppm, 5.1 μB*,

*-70 K), and (-49 ppm, 3.1 μB*, -60 K), respectively.3 We used Eq. (4a) to calculate the

Fermi contact shift of Li, listed in Table I and plotted in Fig. 2, with T=310 K.

*For the GGA case, the calculated values are 131 ppm (Mn), 118 ppm (Fe), 73 ppm *

*(Co) and -63 ppm (Ni), respectively. The calculated value for Li in LiNiPO*4 is negative

and only a little smaller (i.e. larger in absolute value) than the experimental one. On the

contrary, the calculated values of LiMnPO4,LiFePO4 and LiCoPO4 are much larger

than the corresponding experimental ones. In fact, the negative chemical shifts of Li in

LiFePO4 and LiCoPO4 are even predicted to be positive by the GGA calculation. The

*selected results of “GGA+U” method are also listed in Table I and plotted in Fig. 2, and *

are better than those from GGA calculation. For example, the calculated Fermi contact

shift of Li in LiNiPO4* are -53 ppm (with Ueff=0.1 Ry) and -40 ppm (with Ueff*=0.3 Ry),

*respectively, which are close to the experimental values. This implies that the U term *

positive Fermi contact shift of LiMnPO4* is decreased with the increase of Ueff and *

*consequently the agreement between calculation and experiment is improved. *

*However, for Ueff=0.5 Ry, the calculated value is about 93ppm, which is still larger than *

*the experimental value of 68ppm. Better agreement with experiment can be obtained *

*using even larger Ueff *(0.7Ry~1.0Ry), but this is over the values commonly accepted for

transitional metal ions. For LiFePO4 and LiCoPO4, the calculated Fermi contact shifts

*are also decreased with the increase of Ueff*, but they are still positive, even when very

*large Ueff* is used in the calculation. An important result is therefore that we cannot get a

*negative Fermi contact shift for Li in these two compounds with GGA+U calculations. *

*No improvement over the GGA+U method can be obtained when partial exact *

exchange potential is added to the transition-metal ions only (HyF1). From Table I and

*Fig. 2, we find that the result of HyF1 calculation is similar to that of GGA+U: the best *

agreement with experiment can be obtained in LiNiPO4, then LiMnPO4, while the

(experimentally negative) Fermi contact shifts in LiFePO4 and LiCoPO4 are still

predicted to be positive. In contrast, obvious improvement can be obtained with the

HyF2 method. Now the positive Fermi contact shift of Li ion in LiMnPO4 decreases

largely with the increase of exact exchange potential, and good agreement with

experiment can be obtained when ~35% of exact exchange potential (mixing parameter

α=0.35) is added. The negative value of LiNiPO4 increases slowly (smaller absolute

value) when a large portion of exact exchange potential is added, and a pretty good

agreement with experiment is also obtained with a mixing parameter α≈0.35. The most

Fermi contact shifts are now predicted by the HyF2 calculations with the appropriate

*portion of exact exchange potential: it is about -2 ppm with α≈0.5 for LiFePO*4 and

*-21 ppm with α≈0.35 for LiCoPO*4. However, these negative values do not decrease

monotonously with an increase of exact exchange potential, as can be seen from the

results of α=0.35 and 0.5. We propose that the difference between HyF2 and HyF1

methods for the Fermi contact calculation can be understood as follows. Though the

*SIE deficiency in GGA is generally strong for localized d or f orbitals, it should also *

*have some influence on other orbitals, such as O-2p ones. These influences may be tiny *

on the calculation of common quantities, such as total energy and magnetic moment,

and can be omitted in the corresponding calculation. However, for a quantity sensitive

to neighboring environment, such as Fermi contact shift, these influences can not be

omitted. Thus, to improve the results of the Fermi contact shift calculations, the

*addition of partial exact exchange potential is also needed for the O-2p orbitals. From *

*the calculated Fermi contact shifts of Olivine LiMPO*4 compounds with HyF2 method,

we find that the best agreement with experiment can be obtained when mixing

parameter α is about 0.35 except for LiFePO4. The calculated Fermi contact shift of Li

in LiFePO4 is about 9 ppm when α=0.35 (-8 ppm experimentally). Though they have

opposite signs, the difference between the calculated and experimental values is not

large, and we can conclude that a mixing parameter α=0.35 is globally appropriate to

*calculate the Fermi contact shift of Li ions in Olivine LiMPO*4 compounds.

The spin polarized density of states (DOS) and magnetic moment on transition metal

Fig. S-1), showing that the expected transition metal spin states mentioned above are

obtained whatever the calculation. It is interesting to note that the distortion of the TM

*octahedra is strong enough to induce a separation in energy within the t*2g orbitals. This

*can be seen from the projected DOS on Co-3d orbitals in LiCoPO*4 in the

supplementary information Fig. S-2 and S-3, where two spin-down electrons mainly

*occupy spin-down dxz and dyz orbitals and leave the spin-down dxy orbital empty. This is *

an important fact for analyzing the electron spin density transfer mechanisms, as will be

illustrated in subsequent reports.

There is obvious difference between the theoretical (spin-only) and experimental

*effective magnetic moments of LiMPO*4, especially for LiFePO4 and LiCoPO4.3 In

order to consider whether the orbital magnetic moment that may contribute to this

difference can affect the Fermi contact shift on Li ions, we also performed the GGA or

*GGA+U calculation including spin-orbital coupling (SO). The result can be found in *

the supplementary information Table S-III: the difference of Fermi contact shift of Li

obtained by calculation with and without spin-orbital coupling is negligible for

*LiMPO*4. Similar conclusion can also be found in the Li6CoO4 case discussed in the

following section.

B. Study of the Li6CoO4 phase

The space group of Li6CoO4 is tetragonal P42/nmc. The crystal structure contains

CoO4 tetrahedra and two different types of Li sites: Li(1) and Li(2), where the Li(1)O4

(Fig. 3). The Li(1)O4 tetrahedron shares one edge and two corners with CoO4

tetrahedra, while the Li(2)O4 tetrahedron shares its four corners with four CoO4

tetrahedra. The lattice parameters of Li6CoO4 were fully relaxed with VASP (GGA)

*using the experimental ones as a starting point (a=6.536 Å and c=4.654 Å).*53 Co2+ ions

in Li6CoO4 *are in e4t23 configuration (S=3/2). Some of us have recorded *7Li NMR

spectra showing two isotropic signals corresponding to the two Li sites: one is strongly

positive (885 ppm) and the other is strongly negative (-232 ppm). In this study, the

electronic structure of Li6CoO4 was also calculatedusing the VASP code to help in the

interpretation of NMR experimental results.8 However, because the spin density near

the Li nucleus or the HFF is not currently accessible in VASP, the net spin inside

spheres around each Li ion (calculated by integrating the spin density inside those

spheres) was used for interpreting the Fermi contact shift. With this method, the

positive and negative shifts were unambiguously assigned to Li(2) and Li(1),

respectively, but the calculated Li(2)/Li(1) net spin ratio was largely different from the

experimental Fermi contact shifts ratio. Indeed, the experimental Fermi contact shift

ratio Li(2)/Li(1) is close to 3.8 (in absolute value), whereas the spin densities calculated

*with GGA in a 0.6 Å radius sphere yield a much larger ratio of 14.8. With GGA+U *

method, the Li(2)/Li(1) absolute spin density ratio was lowered (12.2), but it is still

much larger than that of the NMR shifts.

The Fermi contact shifts of Li6CoO4 is calculated using Eq. (4a) and considering the

*experimental Weiss constant of -8 K and the effective magnetic moment of 4.1 μB*.54 .

as determined by standardization.19_{ The results are given in Table I and shown in Fig. 4. }

With GGA calculation, the calculated Fermi contact shifts on Li(1) and Li(2) are about

*-176 ppm and 1441 ppm, respectively. Both values have the correct sign, i.e. similar to *

*the corresponding experimental ones (-232 ppm, and 885 ppm), but the calculated shift *

for Li(2) is too large and for Li(1) it is not enough negative. Consequently, while the

calculated ratio between those two values has been improved compared to previous

calculations,8 it is still too large (in absolute value) compared to the experimental one

*(8.2 against 3.8 respectively). Applying “GGA+U” method to Co-3d electrons, the *

positive Fermi contact shift on Li(2) is decreased, and a better agreement with the

experiment is obtained. However, the negative Fermi contact shift on Li(1) is also

decreased (in absolute value), so that the difference between calculation and

experiment is even larger than in the GGA case. Therefore, the ratio between the

calculated NMR shifts of Li(2) and Li(1) is still far from the experimental one whatever

*the Ueff* term introduced in the calculation: 8.1, 9.9, and 7.2 (in absolute value) with

*U*eff*=0.1, 0.3 and 0.5 Ry, respectively. Just like for the LiMPO*4 compounds, adding

*partial exact exchange potential for the Co-3d orbitals (HyF1) has an effect similar to *

*the GGA+U method: both the positive and negative NMR shifts are weakened *

compared to the pure GGA functional. Consequently, only the Fermi contact shift

calculation on Li(2) can be improved, while a worse disagreement with experiment is

obtained for the negative shift of Li(1). On the other hand, if we add partial exact

*exchange potential to both Co-3d and O-2p orbitals (HyF2), a good agreement with *

value on Li(1) is enlarged, leading to a much improved global agreement. The best

agreement with experiment for both Li(1) and Li(2) can be obtained when about 15% of

the GGA exchange potential is replaced by the corresponding exact potential:

941(Li(2)) and -265(Li(1)) with a ratio close to 3.5 (in absolute value). To check the

validity of each of these calculations, we also plotted the spin-polarized DOS and

computed the magnetic moment on Co (in supplementary information Table S-II and

Fig. S-4), which shows that Co2+ (e4 t23) is obtained in each case. To summarize this

part and as already observed for the olivine phases, the anionic p states play an

important role in the polarization mechanism and therefore have to be corrected from

the SIE using a hybrid scheme.

C. Study of the Li3*M*2(PO4)3* (M=V, Fe)*phases

The two Li3Fe2(PO4)3 and Li3V2(PO4)3 phases are isostructural with a monoclinic cell

(P21/n space group). The lithium ions are distributed in three distinct sites: Li(1), Li(2)

*and Li(3) (Fig. 5). Here we use the nomenclature adopted by Patoux et al.*55 Li (1) is in

*a tetrahedral site sharing edges with two MO*6 octahedra; Li(2) is in a distorted trigonal

*bipyramid site sharing respectively an edge and a face with two MO*6 octahedra; finally,

Li(3) is also in a distorted trigonal bipyramid site sharing respectively a face and two

corners with three MO6 octahedra. There are two non symmetry related positions of Fe

or V in Li3*M*2(PO4)3. They occupy distorted octahedral sites with the following

configurations: HS Fe3+(t2g3eg2) and V3+(t2g2eg0). The 7Li MAS NMR spectra of

Li3Fe2(PO4)3 have been measured by some of us with the observation of three distinct

simultaneously obtained by Davis et al.7_{ The }7_{Li NMR spectrum of Li}

3V2(PO4)3 have been recorded by Cahill et al. and exhibits three isotropic signals at 103 ppm, 52 ppm

and 17 ppm, respectively.6 The unambiguous assignment of NMR signals to the three

distinct Li sites is however not obvious due to the complicated crystalline structures and

the small differences observed between those NMR signals. For instance, in the case of

the Li3Fe2(PO4)3 phase, Davis et al. proposed the following ranking for the three Li

*NMR peaks: δ (Li3) > δ (Li1) > δ (Li2), based on the structural analysis,*7 while Kim et

*al. gave a different assignment using calculations based on the Crystal06 code: δ (Li1) *

*> δ (Li2) > δ (Li3).*17 For the Li3V2(PO4)3 phase, Cahill et al. proposed a ranking similar

to the one suggested by Davis et al. on Li3Fe2(PO4)3* i.e. δ (Li3) > δ (Li1) > δ (Li2).*6 In

our previous paper where the VASP code is used for interpreting the NMR Fermi

contact shift, different attributions were proposed for these two compounds.10

Effectively, as in the case of Li6CoO4, the HFF or spin density near the Li nucleus was

not directly accessible. Consequently, the net spin (or integrated spin amount) inside

spheres around each Li ion was used to represent the Fermi contact shift. For

Li3Fe2(PO4)3*, these calculations led to the following assignments: δ (Li1) > δ (Li3) > *

*δ(Li2), whatever the method (GGA or GGA+U) or the radius of the integration sphere, *

with rather close expected shifts for Li(3) and Li(2). For Li3V2(PO4)3, the relative net

*spins calculated around each Li ion depend strongly on the method (GGA or GGA+U) *

used, and within a given method depend very slightly on the radius size. The GGA

*method leads to the following assignment δ (Li3) > δ (Li2) > δ (Li1), whereas GGA+U *

radius size and the U value. These results are therefore different from those of Davis et

al. or Cahill et al. To further study this question we recalculated the Fermi contact shift

of these three Li ions using the WIEN2k approach discussed in the present paper. For

Li3Fe2(PO4)3, we have used the experimental effective magnetic moment (5.89 µB) and

the Weiss constant (-55 K)56 to do the calculation (Eq. (4a)), considering 320 K as the

sample temperature. The results are presented in Table I and shown in Fig. 6a. The

GGA calculated Fermi contact shifts of Li(1), Li(2) and Li(3) in Li3Fe2(PO4)3 are thus

*391 ppm, 222 ppm and 196 ppm (δ (Li1) > δ (Li2) > δ(Li3)), respectively. Adding a U *

term or replacing partial GGA exchange-potential with exact exchange potential on

*Fe-3d orbitals decreases these values and maintains the ranking among them, but the *

corresponding results are still larger than the experimental values. When partial exact

*potential is added to both Fe-3d and O-2p orbitals, the situation gets better as we have *

encountered for the other systems discussed above. There is a reasonable agreement

*with experiment when about 20% of GGA exchange potential of Fe-3d and O-2p *

orbitals is replaced by exact potential. With this adjustment, the three signals 189 ppm,

89 ppm and 39 ppm can be assigned to Li(1), Li(2) and Li(3), respectively. The

assignment we now propose is therefore different from that obtained with our previous

calculations.10 This difference can be explained by analyzing the evolution of the

averaged spin density inside the different atomic spheres. The values reported in Fig. 7a

*are those obtained by the present WIEN2k calculations with the GGA and GGA+U *

*with a Ueff=3 eV (this Ueff=3 eV or 0.22 Ry was one of the Ueff *values used in Ref. 10).

small radius (about R<0.45 Å), the averaged spin density on Li(2) is larger than that on

Li(3), while at larger radii (R>0.45 Å), the averaged spin density on Li(2) becomes the

smallest one. In these previous calculations the radii selected for the analysis were

above the crossing point value (between 0.6 Å, and 0.8 Å); this explains the ranking

*that was proposed: δ(Li1) > δ(Li3) > δ(Li2). Furthermore, this ranking was supported *

by a detailed analysis of the local configuration for each Li site based on the possible

overlap of the Li 2s orbital with idealized 3d orbitals of Fe3+ containing the electron

spins. Note, however, that the relative positions of Li(2) and Li(3), both from the

geometry analysis and the calculations, were considered rather close, as confirmed by

the present results in figure 7a. In the present paper, using the HFF approach (Eq. (4a))

to calculate the Fermi contact shift, we now get an assignment consistent with that by

Kim et al.17* (δ (Li1) > δ (Li2) > δ(Li3)) with however a better agreement with *

experimental results.

Turning to the vanadium phase, the experimental molar magnetic susceptibility of

Li3V2(PO4)3 at the temperature of the NMR experiment is about 0.006emu/mol.57

*However, the number of V ions is 2NA*/mole, so the magnetic susceptibility used in the

calculation is half of the experimental value. In GGA calculation, the Fermi contact

shifts on Li(1), Li(2) and Li(3) ions are 135 ppm, 40 ppm and 65 ppm, respectively and

*the ranking of Fermi contact shifts is δ(Li1) > δ(Li3) > δ(Li2) (see Table I and Fig. 6b). *

*Adding partial exact exchange potential or U term (GGA+U) to Fe-3d orbitals *

decreases these values, especially that on Li(3). So the calculated Fermi contact shift on

*δ(Li3). The best agreement with experimental NMR shifts is again obtained for the *

*HyF2 calculation with 20% GGA exchange potential on V-3d and O-2p orbitals *

replaced by exact exchange potential. Consequently, the three experimental peaks of

103 ppm, 52 ppm and 17 ppm can be assigned to Li(1), Li(2) and Li(3) ions,

respectively. This is in agreement with our earlier local geometry analysis that we were

not able to confirm using DFT/VASP calculations.10 The reason of this difference can

be analyzed as above for Li3Fe2(PO4)3 looking at the evolution of the average spin

density as a function of the sphere radii (see Fig. 7b). When increasing the sphere radius

for the integration, we indeed observe the occurrence of crossing points (≈ 0.5-0.6 Å) where Li(2) and Li(3) average spin densities become larger than the Li(1) one.

Furthermore, the choice of the functional also determines the existence of a crossing

point for Li(2) and Li(3). This clearly demonstrates the limitations of the qualitative

method that was previously used for interpreting the NMR Fermi contact shift. In any

cases, the best agreement with experiment is obtained for both Li3Fe2(PO4)3 and

Li3V2(PO4)3 when 20% GGA exchange potential is replaced by exact exchange

potential.

The spin polarized density of states (DOS) and magnetic moment on transition metal

ions for all Li3Fe2(PO4)3 and Li3V2(PO4)3 calculations are given in supplementary

information Table S-II and Fig. S-5. In Li3V2(PO4)3*, there are two t2g* electrons for the

*three t2g orbitals. Our previous calculation with VASP showed that the three t2g* orbitals

are all partially occupied in GGA calculation, but only two orbitals are occupied in

*To confirm these results, we also plotted the partial V-3d DOS with *

*GGA+U(U*eff=3eV), (see supplementary information Fig. S-6).

IV. CONCLUDING REMARKS

In order to reproduce the experimental results, we have calculated the 7Li ion Fermi

contact shift in several Li paramagnetic compounds with first principle calculations

based on DFT. By studying different structural types or electronic configurations for

the transition metal ions, we came to the conclusion that the calculated Fermi contact

shift is very much dependant of the exchange correlation potential used in the

calculation. Indeed, GGA generally overestimates the spin delocalization mechanism,

*and on the contrary, underestimates the polarization effects. By using GGA+U or *

hybrid functional method, one can reasonably well decrease the overestimation for the

first mechanism but the best agreement with experiment can only be obtained when

*partial exact exchange potential is added to both transition metal 3d and O-2p orbitals. *

The appropriate weight of exact exchange potential in the total exchange potential

depends to some extent on the compound, but our calculations show that the same value

can be used in similar compounds to get a reasonable Fermi contact shift (≈35% for
*LiMPO*4, ≈15% Li6CoO4 for and ≈20% for Li3*M*2(PO4), respectively). These results
help us to assign the peaks of Li ions Fermi contact shift to different Li sites

quantitatively.

From the present work, we can conclude that the F(L)APW method, as implemented

in the WIEN2k code, is particularly well adapted to provide the accurate HFF quantities

compared to the different approaches that have been recently proposed in the literature

for carrying out similar calculations. Among those advantages, we can recall the benefit

of using an auto-adjustable basis set that is accurate enough, and at no additional

computational cost, to provide a very precise spin density at the nucleus. Compared to a

pseudo-potential/plane wave basis set for which the core state relaxation is not yet fully

supported or even implemented or the usage of an LCAO one for which a large basis set

and lot of experience and testing is needed before reaching convergence of the HFF, we

evidence that the (L)APW basis is particularly well designed and efficient for

calculating nuclear-related properties. Furthermore, the judicious way the calculation

of exact potential is implemented in the WIEN2k code allowed us to use hybrid

functional approaches on large systems without any significant additional

computational cost.

ACKNOWLEDGMENTS

This work benefited from a grant from Agence Nationale de la Recherche

(ANR-09-BLAN-0186-01). The Mésocentre de Calcul Intensif Aquitain (MCIA) and

References:

1 M. Whittingham, Chem. Rev. **104, 4271 (2004). **

2 **B. Gee, C. Horne, E. Cairns, and J. Reimer, J. Phys. Chem. B 102, 10142 (1998). **

3 M. Tucker **et al., J. Am. Chem. Soc. 124, 3832 (2002). **

4 **Y. Lee and C. Grey, J. Phys. Chem. B 106, 3576 (2002). **

5 **C. Grey and N. Dupre, Chem. Rev. 104, 4493 (2004). **

6 **L. Cahill, R. Chapman, J. Britten, and G. Goward, J. Phys. Chem. B 110, 7171 (2006). **

7 **L. J. M. Davis, I. Heinmaa, and G. R. Goward, Chem. Mater. 22, 769 (2010). **

8 **D. Carlier, M. Menetrier, and C. Delmas, J. Phys. Chem. C 114, 4749 (2010). **

9 **D. Carlier, M. Menetrier, C. Grey, C. Delmas, and G. Ceder, Phys. Rev. B 67, 174103 **

(2003).

**10 A. Castets, D. Carlier, K. Trad, C. Delmas, and M. Menetrier, J. Phys. Chem. C 114, **
19141 (2010).

**11 I. Bertini, C. Luchinat, and G. Parigi, Prog. Nucl. Magn. Reson. Spectrosc. 40, 249 **
(2002).

**12 S. Blügel, H. Akai, R. Zeller, and P. Dederichs, Phys. Rev. B 35, 3271 (1987). **
**13 H. Ebert, R. Zeller, B. Drittler, and P. Dederichs, J. Appl. Phys. 67, 4576 (1990). **
**14 P. Novak, J. Kunes, W. Pickett, W. Ku, and F. Wagner, Phys. Rev. B 67, 140403 (2003). **
**15 G. Mali, A. Meden, and R. Dominko, Chem. Commun. 46, 3306 (2010). **

16 G. Mali, M. Rangus, C. Sirisopanaporn, and R. Dominko, Solid State Nucl. Magn. Reson.

**42, 33 (2012). **

17 J. Kim **et al., J. Am. Chem. Soc. 132, 16825 (2010). **

18 A. Castets **et al., Solid State Nucl. Magn. Reson. 42, 42 (2012). **

19 A. Castets **et al., J. Phys. Chem. C 115, 16234 (2011). **

**20 C. Bauschlicher, S. Langhoff, H. Partridge, and D. Chong, J. Chem. Phys. 89, 2985 **
(1988).

**21 C. Bauschlicher, J. Chem. Phys. 92, 518 (1990). **

**22 S. Perera, J. Watts, and R. Bartlett, J. Chem. Phys. 100, 1425 (1994). **
**23 S. Fau and R. Bartlett, J. Phys. Chem. A 107, 6648 (2003). **

**25 N. Ishii and T. Shimizu, Phys. Rev. A 48, 1691 (1993). **

**26 M. Munzarova and M. Kaupp, J. Phys. Chem. A 103, 9966 (1999). **

**27 L. Hermosilla, P. Calle, J. de la Vega, and C. Sieiro, J. Phys. Chem. A 109, 1114 (2005). **
**28 R. Batra, B. Giese, M. Spichty, G. Gescheidt, and K. Houk, J. Phys. Chem. 100, 18371 **
(1996).

**29 C. Adamo, V. Barone, and A. Fortunelli, J. Phys. Chem. 98, 8648 (1994). **

**30 L. Eriksson, V. Malkin, O. Malkina, and D. Salahub, J. Chem. Phys. 99, 9756 (1993). **
**31 S. Larsen, J. Phys. Chem. A 105, 8333 (2001). **

**32 E. S. Kadantsev and T. Ziegler, Magn. Reson. Chem. 48, S2 (2010). **
**33 M. Bahramy, M. Sluiter, and Y. Kawazoe, Phys. Rev. B 73, 045111 (2006). **

**34 H. Ebert, H. Winter, B. Gyorffy, D. Johnson, and F. Pinski, J. Phys. F: Met. Phys. 18, 719 **
(1988).

**35 P. Novak and V. Chlan, Phys. Rev. B 81, 174412 (2010). **
**36 C. Vandewalle and P. Blöchl, Phys. Rev. B 47, 4244 (1993). **
**37 P. Blöchl, Phys. Rev. B 50, 17953 (1994). **

**38 M. Marsman and G. Kresse, J. Chem. Phys. 125, 104101 (2006). **

**39 M. S. Bahramy, M. H. F. Sluiter, and Y. Kawazoe, Phys. Rev. B 76, 035124 (2007). **
**40 O. Yazyev, I. Tavernelli, L. Helm, and U. Rothlisberger, Phys. Rev. B 71, 115110 (2005). **
**41 V. Anisimov, J. Zaanen, and O. Andersen, Phys. Rev. B 44, 943 (1991). **

**42 A. Becke, J. Chem. Phys. 98, 1372 (1993). **

*43 P. Blaha, K. Schwarz, G. K. H. Madsen, D. Kvasnicka, and J. Luitz, WIEN2k, An *

*Augmented Plane Wave + Local Orbitals Program for Calculating Crystal Properties (K.-H. *

Schwarz (Technische Universität, Austria), 2001).

**44 G. Kresse and J. Furthmuller, Comput. Mater. Sci. 6, 15 (1996). **
**45 G. Kresse and D. Joubert, Phys. Rev. B 59, 1758 (1999). **
**46 G. Kresse and J. Furthmuller, Phys. Rev. B 54, 11169 (1996). **

**47 J. P. Perdew, K. Burke, and M. Ernzerhof, Phys. Rev. Lett. 77, 3865 (1996). **
48 Y. S. Zhang, D. Carlier, M. Menetrier, and F. Boucher, to be submitted (2012).
**49 V. Anisimov, I. Solovyev, M. Korotin, M. Czyzyk, and G. Sawatzky, Phys. Rev. B 48, **
16929 (1993).

50 O. Garcia-Moreno **et al., Chem. Mater. 13, 1570 (2001). **

**51 G. Rousse, J. Rodriguez-Carvajal, S. Patoux, and C. Masquelier, Chem. Mater. 15, 4082 **
(2003).

**52 F. Kubel, Z. Kristallogr. 209, 755 (1994). **

**53 R. Luge and R. Hoppe, Z. Anorg. Allg. Chem. 534, 61 (1986). **
**54 A. Moller, Chem. Mater. 10, 3196 (1998). **

**55 S. Patoux, C. Wurm, M. Morcrette, G. Rousse, and C. Masquelier, J. Power Sources 119, **
278 (2003), 11th International Meeting on Lithium Batteries, MONTEREY, CALIFORNIA,
JUN 24-28, 2002.

**56 G. Rousse, J. Rodriguez-Carvajal, C. Wurm, and C. Masquelier, Chem. Mater. 13, 4527 **
(2001).

**57 L. S. Cahill, R. P. Chapman, C. W. Kirby, and G. R. Goward, Appl. Magn. Reson. 32, 565 **
(2007).

Table I. Comparison of experimental Fermi contact shifts (ppm, in bold) with the
calculated ones obtained for various compounds with different functionals using
*either Eqs. (4a) or (4b) (see text). For the GGA+U, the effective potential (U*eff) is
given in Ry and for the hybrid functionals (HyF1 of HyF2) mixing parameters are
reported

*Compound Site GGA GGA+U (Ueff) HyF1(α) HyF2(α) * **Exp**
0.10 0.30 0.50 0.10 0.35 0.50 0.10 0.35 0.50
LiMnPO4 Li 131 120 105 93 125 90 112 107 56 24 **68**
LiFePO4 Li 118 85 68 58 92 70 65 59 9 -2 **-8**
LiCoPO4 Li 73 39 31 27 36 26 24 8 -21 -20 **-86**
LiNiPO4 Li -63 -53 -40 -30 -62 -22 -15 -60 -44 -33 **-49**
0.10 0.30 0.50 0.10 0.15 0.30 0.10 0.15 0.30
Li6CoO4
Li(1) -176 -160 -103 -110 -152 -142 -90 **-242 -265 -307 -232**
Li(2) 1441 1300 1025 793 1198 1080 765 1092 941 605 **885**
0.10 0.30 0.50 0.10 0.20 0.25 0.10 0.20 0.25
Li3Fe2(PO4)3
Li(1) 391 363 307 259 360 333 320 306 229 196 **189**
Li(2) 222 174 165 137 199 179 170 149 86 58 **89**
Li(3) 196 172 143 113 173 153 142 118 49 18 **39**
0.10 0.22 0.30 0.10 0.20 0.25 0.10 0.20 0.25
Li3V2(PO4)3
Li(1) 135 138 128 122 129 131 129 97 104 99 **103**
Li(2) 40 46 33 29 45 39 37 58 50 43 **52**
Li(3) 65 36 30 27 33 17 14 37 24 16 **17**

FIGURE CAPTIONS

*FIG. 1. (Color online) Environment of Li atoms in LiMPO*4. The LiO6 octahedron
*shares edges with two MO*6* octahedra and corners with four other MO*6 polyhedra.

FIG. 2. (Color online) Comparison of experimental Fermi contact shifts of Li in
*olivine LiMPO*4* (M = Mn, Fe, Co, Ni) with the calculated ones obtained with different *
*approaches using Eq. (4a) (T = 310K). For the GGA+U, the effective potential (U*eff)
is given in Ry and for the hybrid functionals (HyF1 of HyF2, see text) mixing
parameters are reported: a = 0.35 (Mn, Co, and Ni); a = 0.5 (Fe).

FIG. 3. (Color online) Environment for the two Li sites of Li6CoO4 showing the local geometry: (a) Li(1); (b) Li(2).

*FIG. 4. (Color online) Comparison of experimental Fermi contact shifts of Li(1) and *
Li(2) in Li6CoO4 with the calculated ones obtained with different approaches using Eq.
*(4a) (T = 320K). For the GGA+U, the effective potential (U*eff) is given in Ry and for
*the hybrid functionals (HyF1 of HyF2, see text) mixing parameters are reported. *

FIG. 5. (Color online) Environment for the three Li sites of Li3V2(PO4)3 showing the local geometry: (a) Li(1); (b) Li(2); (c) Li(3).

*FIG. 6. (Color online) Comparison of experimental Fermi contact shifts of Li(1), *
Li(2), and Li(3) in Li3*M*2(PO4)3* (M = Fe (a); V (b)) with the calculated ones obtained *
with different approaches using Eqs. (4a) or (4b) (see text, T = 320K). For the
*GGA+U, the effective potential (U*eff) is given in Ry and for the hybrid functionals
*(HyF1 of HyF2, see text) mixing parameters are reported. *

FIG. 7. (Color online) Average spin density around the three Li nuclei for
Li3Fe2(PO4)3 (a) and Li3V2(PO4)3 (b) as a function of the integration sphere radius.
*Results are given for the GGA and GGA+U (U*eff = 3eV) calculations.

*FIG. 1. (Color online) Environment of Li atoms in LiMPO*4. The LiO6 octahedron
*shares edges with two MO*6* octahedra and corners with four other MO*6 polyhedra.

FIG. 2. (Color online) Comparison of experimental Fermi contact shifts of Li in
*olivine LiMPO*4* (M = Mn, Fe, Co, Ni) with the calculated ones obtained with different *
*approaches using Eq. (4a) (T = 310K). For the GGA+U, the effective potential (U*eff)
is given in Ry and for the hybrid functionals (HyF1 of HyF2, see text) mixing
parameters are reported: a = 0.35 (Mn, Co, and Ni); a = 0.5 (Fe).

FIG. 3. (Color online) Environment for the two Li sites of Li6CoO4 showing the local geometry: (a) Li(1); (b) Li(2).

*FIG. 4. (Color online) Comparison of experimental Fermi contact shifts of Li(1) and *
Li(2) in Li6CoO4 with the calculated ones obtained with different approaches using Eq.
*(4a) (T = 320K). For the GGA+U, the effective potential (U*eff) is given in Ry and for
*the hybrid functionals (HyF1 of HyF2, see text) mixing parameters are reported. *

FIG. 5. (Color online) Environment for the three Li sites of Li3V2(PO4)3 showing the local geometry: (a) Li(1); (b) Li(2); (c) Li(3).

*FIG. 6. (Color online) Comparison of experimental Fermi contact shifts of Li(1), *
Li(2), and Li(3) in Li3*M*2(PO4)3* (M = Fe (a); V (b)) with the calculated ones obtained *
with different approaches using Eqs. (4a) or (4b) (see text, T = 320K). For the
*GGA+U, the effective potential (U*eff) is given in Ry and for the hybrid functionals
*(HyF1 of HyF2, see text) mixing parameters are reported. *

FIG. 7. (Color online) Average spin density around the three Li nuclei for
Li3Fe2(PO4)3 (a) and Li3V2(PO4)3 (b) as a function of the integration sphere radius.
*Results are given for the GGA and GGA+U (U*eff = 3eV) calculations.